## E

## ﬀ

## ects of Dynamical Electron Di

## ﬀ

## raction on Phase Shift Detected by Electron

## Holography

### Zentaro Akase

1,2### and Daisuke Shindo

1,21_{Institute of Multidisciplinary Research for Advanced Materials, Tohoku University, Sendai 980-8577, Japan}
2_{Center for Emergent Matter Science, RIKEN, Wako 351-0198, Japan}

Recently, the eﬀect of dynamical electron diﬀraction on the phase shift in electromagnetic ﬁeld analysis using transmission electron microscopy has become increasingly important. In the present study, we investigated the eﬀect of dynamical electron diﬀraction on the phase shift in electron holograms recorded from a wedge-shaped specimen of single-crystal Si around a Bragg diﬀraction condition. The results show that the eﬀective inner potential depends on the direction of the incident electron beam, especially near Bragg conditions. The characteristic phase shift was analyzed using dynamical electron diﬀraction theory (Bethe method). [doi:10.2320/matertrans.MT-MI2019007]

(Received April 26, 2019; Accepted August 5, 2019; Published August 30, 2019)

Keywords: dynamical electron diﬀraction, phase shift, electron holography

1. Introduction

With recent improvements in the precision and sensitivity

of electromagneticﬁeld analysis using transmission electron

microscopy, such as electron holography,13) DCP-STEM4)

and electron diﬀractive imaging,5) the eﬀect of dynamical

electron diﬀraction on the phase shift º has become

important. Generally, the phase shift of an electron beam

passing through an electrical potential ¤is described by

ºðx; yÞ ¼·

Z

¤ðx; y; zÞdz ð1Þ

where the interaction constant·is given by

· ¼ 2³

Eð1þpﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ1¢2Þ

where¢=¯/c,Eis the accelerating voltage,is the electron

wavelength, ¯ is the electron velocity and c is the light

velocity.6)In calculating the phase shift of an electron passing

through a specimen, the mean inner potential V0 of the

specimen can be used instead of ¤ when the eﬀect of the

electron diﬀraction is weak.7,8) However, when the eﬀect of

the electron diﬀraction is large, for example, when the

specimen exhibits large bending (many bend contour lines

appear on the bright-ﬁeld image) or a polycrystalline

structure with grains of random orientation, it is diﬃcult to

apply eq. (1). In that case, the dynamical electron diﬀraction

should be taken into account because kinematical diﬀraction

theory cannot be used near Bragg diﬀraction. In previous

research, the dynamical diﬀraction eﬀect on the phase shift

was discussed using the two-beam approximation,911) and

inner potentials were determined by multi-beam dynamical

diﬀraction theory.12) The dynamical diﬀraction eﬀect of

diﬀracted beam for the dark-ﬁeld electron holography was

also discussed.13) In our research, we recorded holograms

from a wedge-shaped specimen of single-crystal Si around

a Bragg diﬀraction condition. We discuss the characteristic

phase shifts of the transmitted beam, which appear in the reconstructed phase images, as functions of thickness and

specimen tilt using multi-beam dynamical electron diﬀraction

theory, in order to understand how dynamical diﬀractions

aﬀect the phase shift through a quantitative interpretation

with high accuracy.

2. Method

2.1 Calculation of phase shift with dynamical theory of electron diﬀraction

For the phase shift of an electron beam, the solution of the

HowieWhelan equations14)_{for the two-beam approximation}

of dynamical theory gives a qualitative solution. Near the

Bragg condition, two Bloch waves with slightly diﬀerent

wavelengths are excited, and the excitation rate depends on the incident beam direction. However, the solution of the

HowieWhelan equation includes many approximations

ignoring phase terms to ensure intensity, and we therefore

selected to use the Bethe method,1522)which is a multi-beam

dynamical diﬀraction theory, for a quantitative analysis of the

phase shift.

According to the dynamical theory of electron diﬀraction

(Bethe method), the wave function ¼0 of a transmitted

electron beam (which corresponds to the object wave in the

term of electron holography) that propagates a distance tin

a crystal specimen is expressed by a linear combination of

Bloch waves, as follows:23)

¼0¼X j

¡ðjÞ_{C}ðjÞ

0 expð2³ijkðjÞjtÞ

¼X

j

¡ðjÞ_{C}ðjÞ

0 expð2³iðjKj þ£ðjÞÞtÞ

¼expð2³ijKjtÞX

j

¡ðjÞ

CðjÞ0 expð2³i£ðjÞtÞ ð2Þ

whereKis the wave vector of an incident beam in the mean

inner potential of the specimen.k( j),C0( j),£( j)and¡( j)are the

wave vector, amplitude of the incident wave (eigenvector),

eigenvalue and excitation coeﬃcient of the j-th Bloch wave,

respectively. The parametersC0( j),£( j)and¡( j)can be solved

from Schrodinger’s equation. When the crystal has a

centrosymmetric structure, ¡( j)_{=}_{C}

0( j). The intensity I0 of

the object wave can then be calculated using the following equation:

I0¼¼0¼0 ¼

X

j

¡ðjÞ_{C}ðjÞ

0 expð2³i£ðjÞtÞ

2

ð3Þ

The phase shiftºis the diﬀerence between the phase of an

object wave (eq. (2)) and the phase of a reference wave. The

phase of the reference wave is expressed by2³jjt, where

is the wave vector of an electron in vacuum. Therefore,ºcan

be calculated using the following formula; º¼anglef¼0expð2³ij»jtÞg

¼angle

"(

expð2³ijKjtÞX

j

¡ðjÞ_{C}ðjÞ

0 expð2³i£ðjÞtÞ

)

expð2³ij»jtÞ

#

¼angle expð2³iðjKj j»jÞtÞX

j

¡ðjÞ_{C}ðjÞ

0 expð2³i£ðjÞtÞ

( )

¼angle exp i·

Z_{t}

0 V0dt

_{ X}

j

¡ðjÞ_{C}ðjÞ

0 expð2³i£ðjÞtÞ

( )

ð4Þ

where angle (x) is a function that outputs the angle of the

complex number x. Comparing eq. (4) with eq. (1), it is

noted that the eﬀect of dynamical electron diﬀraction appears

in the summation term in eq. (4).¡,C0and £depend on the

excitation errors (deviation parameter, the distance between a

reciprocal lattice point and the Ewald sphere)sgof the excited

Bragg reﬂections, i.e. the tilting angle of the specimen.

Hence, it is considered that the phase shift also depends on the tilting angle. Equation (3) and eq. (4) enable us to determine the intensity and phase shift of an object wave

under the eﬀect of dynamical diﬀraction as a function of the

specimen tilting angle and thickness.

To simulate the intensity and phase shift of the transmitted beam, nine beams in a 220 systematic row (000, 220, 440,

660, 880, -2-20, -4-40, -6-60, -8-80) are considered in our

calculations. The eﬀects of absorption of intensity are not

considered. We developed a code to calculate the dynamical

electron diﬀraction using the Bethe method including an

external subroutine that yields the atomic form factors for

electron diﬀraction.24)The value ofV0of Si used in our code

is 11.5 V.25)

2.2 Experimental procedure

A TEM specimen was prepared from a Si (100) wafer using a focused ion beam (FIB) milling system (JIB-45000 MultiBeam, JEOL). The wedge angle, which was controlled by FIB, was about 52°. Electron holography was performed using a 300-kV TEM system (JEM-3000F, JEOL) equipped with a single biprism. The holograms were recorded under a

two-beam condition (transmitted beam and 220 reﬂection).

The incident beam direction was controlled using a beam tilt function.

[image:2.595.52.289.170.328.2]3. Results and Discussion

Figure 1 shows the results of a calculation of the

dynamical theory of electron diﬀraction. The columns (a)

(e) show diﬀerent diﬀraction conditions. The upper row (i)

shows plots of ¼0expð2³ijjtÞ on a complex plane with

thickness as a parameter (refer eq. (4)). The range of the thickness is from 0 nm to 300 nm. The data from 20 nm to 80 nm are plotted by red bold lines. To explain Fig. 1(i), a

blue vector indicating¼0expð2³ijjtÞat 20 nm thickness is

drawn in Fig. 1(a-i). The length of the vector corresponds to

the square root of the intensityI0, and the angle between the

real axis and the vector corresponds to the phase shiftº. The

middle row (ii) and the lower row (iii) show the intensity and

the phase shift plotted as functions of thicknesst.

In the center column (Fig. 1(c)), the specimen is under an

exact 220 Bragg diﬀraction condition. In this condition, the

(a) (b) (c) (d) (e)

(i)

(ii)

(iii)

[image:2.595.71.529.522.751.2]trajectory of ¼0expð2³ijjtÞ intersects the origin of the complex plane, as shown in Fig. 1(c-i). At the thickness of the intersection, the length of the vector is zero, so that the

corresponding position in the bright-ﬁeld image shows a dark

contrast. It is noted that the direction of the¼0expð2³ijjtÞ

vector is turned over by ³across the origin of the complex

plane in Fig. 1(c-i). Therefore, the phase shift proﬁle

(Fig. 1(c-iii)) shows jumps of³at the dark thickness fringes.

In our calculation, those thicknesses are 50.8 nm, 152.0 nm

and 253.2 nm. Those thicknesses become close to (1/2+

n)²220, because the diﬀraction condition is almost two beams

condition. Here, ²220 is the extinction distance of 220

reﬂection, and n is an integer (n²0). In our calculation

²220becomes 108 nm.

The left and right side columns of Fig. 1 show the results

when the sign of the excitation error of the 220 reﬂection

s220is negative and positive, respectively. Figure 1(iii) shows

that the gradient of the phase shift depends on the sign of the

excitation error s220, i.e. when s220<0, the gradient of the

phase-shift is high and when s220>0, the gradient of the

phase-shift is low. This result can be understood by

comparing Fig. 1(b-i) and Fig. 1(d-i). In those ﬁgures, the

trajectory of ¼0expð2³ijjtÞ, shown as red bold lines for

thicknesses from 20 nm to 80 nm, forms a shape of a small

loop. When the sign ofs220is negative (Fig. 1(b-i)), the small

loop includes the origin of the complex plane. This means the

increase of the phase shift is larger than 2³. When s220 is

positive (Fig. 1(d-i)), the small loop does not include the origin of the complex plane, which means the increase of

the phase shift is less than 2³. Thus, eq. (4) explains the

[image:3.595.134.463.330.753.2]characteristic phase shift around the Bragg condition that is not explained by eq. (1).

Figure 2 shows bright-ﬁeld images and reconstructed

phase images of a wedge shape Si specimen, and the phase

shift proﬁles in the region of the specimen indicated by the

red rectangles in the bright-ﬁeld and reconstructed phase

images. The specimen shown in Fig. 2(a) is under a non-Bragg condition and that shown in Fig. 2(b) is under an exact

220 Bragg diﬀraction condition. Under the non-Bragg

condition, there are no thickness fringes in the bright ﬁeld

(a) (b)

image, and the phase shift increases in proportion to the

specimen thickness. Under the exact 220 Bragg diﬀraction

condition, thickness fringes appear in the bright-ﬁeld image,

and the phase shift jumps by³(indicated by red arrows in the

reconstructed phase image and the phase-shift proﬁle) where

the dark thickness fringes appear in the corresponding

bright-ﬁeld image. These ³jumps cannot be explained by eq. (1).

But they can be explained by dynamical theory of electron

diﬀraction as shown in Fig. 1(c).

Next, we systematically tilted the direction of the incident

electron beam around the 220 Bragg diﬀraction condition

using a beam tilt function of the illumination system. The

bright ﬁeld images, the reconstructed phase images and the

phase shift proﬁles for each tilt conditions are shown in

Fig. 3(a)(n). Figures 3(o) and 3(p) are diﬀraction patterns

obtained in the diﬀraction condition of Figs. 3(a) and 3(n),

respectively. From a movement of a cross point of Kikuchi lines indicated by black arrows in Figs. 3(o), (p), the total tilting angle from Fig. 3(a) to 3(n) is estimated to be 5.04 mrad. The tilting was changed in constant steps

(0.39 mrad), such that for the tilting condition of Fig. 3(a)

(g), the excitation error of the 220 reﬂections220is negative

(which means that the reciprocal lattice point of 220 is

located outside the Ewald sphere) and for Fig. 3(h)(n)s220is

positive (the reciprocal lattice point of 220 is located inside the Ewald sphere). It should be noted that the gradient of the phase-shift against specimen thickness depends on the sign of the excitation error as discussed in the simulation part, i.e.,

when s220<0, the gradient of the phase-shift is high and

when s220>0, the gradient of the phase-shift is low. The

[image:4.595.150.450.73.510.2]complicated phase shifts near the thickness of (1/2+n)²220,

which was expected by the simulation, were also observed experimentally.

4. Summary

The complicated phase shifts of an object wave around the

Bragg diﬀraction condition, such as a jump in the phase shift

and an eﬀective inner potential depending on the diﬀraction

conditions, were explained by the dynamical theory of

electron diﬀraction. Near a Bragg condition, many Bloch

waves with slightly diﬀerent wavelengths are excited, and

the excitation rate of each Bloch wave depends on the

incident beam direction. By taking into account the eﬀect

of dynamical electron diﬀraction, the phase-shift map

acquired by TEM methods, such as electron holography,

DCP-STEM and electron diﬀractive imaging, can be

interpreted quantitatively with high accuracy.

Acknowledgements

This work was supported by JSPS Grant-in-Aid for

Scientiﬁc Research No. JP15K06419.

REFERENCES

1) A. Lubk, D. Wolf and H. Lichte:Ultramicroscopy110(2010) 438446.

2) D. Shindo and Y. Murakami:J. Phys. D41(2008) 183002.

3) D. Shindo and Y. Murakami: J. Electron Microsc.60(2011) S225 S237.

4) N. Shibata, S.D. Findlay, Y. Kohno, H. Sawada, Y. Kondo and Y. Ikuhara:Nat. Phys.8(2012) 611615.

5) J. Yamasaki, K. Ohta, S. Morishita and N. Tanaka:Appl. Phys. Lett.

101(2012) 234105.

6) D. Shindo and T. Oikawa: Analytical Electron Microscopy for Materials Science, (Springer-Verlag, Tokyo, 2002).

7) D. Shindo, T. Musashi, Y. Ikematsu, Y. Murakami, N. Nakamura and H. Chiba:J. Electron Microsc.54(2005) 1117.

8) C.-W. Lee, Y. Ikematsu and D. Shindo:Mater. Trans.41(2000) 1129 1131.

9) K. Yada, K. Shibata and T. Hibi:J. Electron Microsc.22(1973) 223 230.

10) G. Ade: Optik62(1982) 6785.

11) K.J. Hanszen:J. Phys. D19(1986) 373395.

12) M. Gajdardziska-Josifovska, M.R. McCartney, W.J. de Ruijter, D.J. Smith, J.K. Weiss and J.M. Zuo: Ultramicroscopy 50 (1993) 285 299.

13) A. Lubk, E. Javon, N. Cherkashin, S. Reboh, C. Gatel and M. Hÿtch:

Ultramicroscopy136(2014) 4249.

14) A. Howie and M.J. Whelan:Proc. R. Soc. A263(1961) 217.

15) H. Bethe:Ann. Phys.392(1928) 55129.

16) C.H. Mac Gillavry:Physica7(1940) 329343.

17) R.D. Heidenreich:J. Appl. Phys.20(1949) 993.

18) N. Kato:J. Phys. Soc. Jpn.7(1952) 397406.

19) L. Sturkey: Acta Crystallogr.10(1957) 858859. 20) F. Fujimoto:J. Phys. Soc. Jpn.14(1959) 1558.

21) H. Niehrs: Z. Naturforsch.14a(1959) 504511. 22) H. Niehrs:Z. Phys.156(1959) 446467.

23) C.J. Humphreys:Rep. Prog. Phys.42(1979) 1825.

24) D.M. Bird and Q.A. King:Acta Crystallogr. Sec. A46(1990) 202208.